Superior Electrochemical Performance of
Electropolymerized Self-Organized TiO2 Nanotubes
Fabricated by Anodization of Ti Grid

Vinsensia Ade Sugiawati, Florence Vacandio, Alina Galeyeva, A. Kurbatov,
Thierry Djenizian

► To cite this version:

Vinsensia Ade Sugiawati, Florence Vacandio, Alina Galeyeva, A. Kurbatov, Thierry Djenizian. Superior Electrochemical Performance of Electropolymerized Self-Organized TiO2 Nanotubes Fabricated by Anodization of Ti Grid. Frontiers in Physics, 2019, 7, 10.3389/fphy.2019.00179. [hal-02649494](https://hal HAL Id: hal-02649494)

HAL Id: hal-02649494

https://amu.hal.science/hal-02649494v1

Submitted on 29 May 2020

**HAL** is a multi-disciplinary open access
archive for the deposit and dissemination of sci-
entific research documents, whether they are pub-
lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.

L'archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d'enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.

<figure><img src="image_1.png" /></figure>

Distributed under a Creative Commons CC BY 4.0 - Attribution - International License
# Superior Electrochemical Performance of Electropolymerized Self-Organized TiO2 Nanotubes Fabricated by Anodization of Ti Grid

Vinsensia A. Sugiawati¹, Florence Vacandio², Thierry Djenizian¹*, Alina Galeyeva³, Andrey P. Kurbatov³*

¹École des Mines de Saint-Étienne - Campus Georges Charpak Provence, France, ²Aix-Marseille Université, France, ³Al-Farabi Kazakhstan National University, Kazakhstan

**Submitted to Journal:**

Frontiers in Physics

**Specialty Section:**

Physical Chemistry and Chemical Physics

**Article type:**

Original Research Article

**Manuscript ID:**

496158

**Received on:**

05 Sep 2019

**Revised on:**

19 Oct 2019

**Frontiers website link:**

www.frontiersin.org
**Conflict of interest statement**

The authors declare that the research was conducted in the absence of any commercial or financial relationships that could be construed as a potential conflict of interest

**Author contribution statement**

VA S performed experiments, analyzed the experimental results and wrote the manuscript. VA S, AG, APK, FV and TD discussed experimental results. FV and TD supervised the works. All the authors contributed to the reading of paper and gave advice on the revision of the manuscript.

**Keywords**

Anode, microbatteries, polymer electrolyte, Ti grid, TiO 2 nanotubes

**Abstract**

Word count: 136

Self-organized TiO2 nanotubes grown on Ti grid acting as anode for Li-ion microbatteries were prepared via an electrochemical anodization. By tuning the anodization time, the morphology and length of the nanotubes were investigated by scanning electron microscope. When the anodization time reached 1.5 h, the TiO2nts/Ti grid anode showed a well-defined nanotubes, which are stable, well adherent ~90 nm with a length of 1.88 µm. Due to their high surface utilization, surface area and material loading per unit area, TiO2nts/Ti grid anode using polymer electrolyte exhibited a high areal capacity of 376 µAh cm-2 at C/10 rate and a stable discharge plateau at 1.8 V without using a polymer binder and conductive additive. The storage capacity of the TiO2nts/Ti grid after 10 cycles is fifteen times higher compared to previous reports using planar Ti foils.

**Contribution to the field**

Dear Professor Galstyan In this work, we report the fabrication of self-organized TiO2 nanotubes grown on Ti grid by anodization. By tuning the anodization time, well-defined nanotubes could be obtained, which are stable and well adherent. Due to their high surface utilization, surface area and material loading per unit area, TiO2nts/Ti grid anode using polymer electrolyte exhibited a high areal capacity of 376 µAh cm-2 at C/10 rate and a stable discharge plateau at 1.8 V without using a polymer binder and conductive additive. More remakbaly, the storage capacity of the TiO2nts/Ti grid after 10 cycles is fifteen times higher compared to previous reports using planar Ti foils. >considering the outstanding performance, we believe that the results could attract the interest of the scientists interested in the development of Li-ion batteries and we hope you can consider the mansucript for potential publication in Frontiers in Physics.

**Ethics statements**

**Studies involving animal subjects**

Generated Statement: No animal studies are presented in this manuscript.

**Studies involving human subjects**

Generated Statement: No human studies are presented in this manuscript.

**Inclusion of identifiable human data**

Generated Statement: No potentially identifiable human images or data is presented in this study.

**Data availability statement**

Generated Statement: The datasets generated for this study are available on request to the corresponding author.
1

2

**Enhanced Electrochemical Performance of Electropolymerized Self-Organized TiO₂ Nanotubes Fabricated by Anodization of Ti Grid**

3

Vinsensia Ade Sugiawati¹, Florence Vacandio², A. Galeyeva³, A. P. Kurbatov³ and Thierry

4

Djenizian¹*

5

6

¹ Mines Saint-Etienne, Center of Microelectronics in Provence, Department of Flexible Electronics, France

7

8

² Aix Marseille Université, CNRS, Electrochemistry of Materials Research Group, MADIREL, UMR 7246, F-13397, Marseille Cedex 20, France

9

³Al-Farabi Kazakh National University, Center of Physical-Chemical Methods of Research and Analysis, Kazakhstan, Almaty, Tole bi str., 96A.

10

11

* Correspondence:

12

Corresponding Author

13

thierry.djenizian@emse.fr

14

**Keywords: Anode, Microbatteries, Polymer electrolyte, Ti grid, TiO₂ nanotubes**

15

16

**Abstract**

17

18

19

20

21

22

23

24

25

Self-organized TiO₂ nanotubes grown on Ti grid acting as anode for Li-ion microbatteries were prepared via an electrochemical anodization. By tuning the anodization time, the morphology and length of the nanotubes were investigated by scanning electron microscope. When the anodization time reached 1.5 h, the TiO₂nts/Ti grid anode showed a well-defined nanotubes, which are stable, well adherent ~90 nm with a length of 1.9 ± 0.1 µm. Due to their high surface utilization, surface area and material loading per unit area, TiO₂nts/Ti grid anode using polymer electrolyte exhibited a high areal capacity of 376 µAh cm⁻² at C/10 rate and a stable discharge plateau at 1.8 V without using a polymer binder and conductive additive. The storage capacity of the TiO₂nts/Ti grid after 10 cycles is fifteen times higher compared to previous reports using planar Ti foils.
## 1. Introduction

Due to their high energy density, no memory effect and long cycle life, rechargeable Li-ion batteries (LIBs) have been extensively used as power sources for many electronic devices [1-4]. More recently, all-solid-state microbatteries have attracted intense attention for powering miniaturized electronics such as wireless sensors and a wide range of applications for the Internet of Things (IoT) [5-8]. Titanium dioxide (TiO₂) is an attractive and versatile material that is used in many technologies due to its unique properties such as high surface area, electronic properties, biocompatibility, and environmental well-being [9,10]. Particularly, synthesis of nanostructured TiO₂ such as nanotubes, nanowires and nanofibers has raised interest lately compared to the conventional microstructures due to their high surface-to-volume ratio [11-13]. The first reports on the formation of self-organized nanotubes on titanium by Assefpour-Dezfuly et al. in 1984 [14] where Ti metal was firstly etched in alkaline peroxide, then anodized in chromic acid and later by Zwilling et al. in 1999 [15] reported on the formation of nanoporous anodized TiO₂ nanotubes in a fluoride containing electrolyte. Since then, TiO₂ nanotubes have been extensively explored in various fields, such as photocatalysis[16], sensors[17], dye sensitized solar cells[18] and energy storage device [19].

Various approaches, such as sol-gel, hydrothermal treatment, template assisted method, electrospinning and electrochemical anodization have been employed to prepare one-dimensional TiO₂ nanostructures [20]. However, self-organized TiO₂nts formed by anodization method is preferred owing to their simplicity, better control over the nanotube morphology and low-cost [19,21]. Thus, pristine as well as chemically modified TiO₂nts obtained by anodization have been used as negative electrodes for high performance Li-ion batteries [22-24]. Most studies on self-organized TiO₂nts are focused on the planar surface, for instance Ti foil. The utilization of Ti grid as the substrate to synthesize the TiO₂nts has been extensively studied owing to its flexibility and unique geometry [25,26]. Much attentions have been paid on the fabrication of the TiO₂nts on Ti grid as photoanode,
possessing an enhanced performance in terms of photon absorption and electron collection efficiency
compared to anodized Ti foil [27–29]. Previous studies have shown the use of TiO2nts /Ti grid in Dye
Sensitized Solar Cells (DSSCs) can effectively improve the charge collection efficiency of
approximately 3.15% [27]. Liu et al. fabricated vertically oriented TiO2 nanotube arrays with
controllable lengths on Ti grids by electrochemical anodization in ethylene glycol-based electrolyte
and investigated their potential application as flexible electrodes for DSSCs [30]. The work reported
by Motola et al. showed a high photocatalytic, antimicrobial and antibioflm activities of the TiO2
nanotube layers grown on Ti grid [31,32].

Despite a large number of reports published on the fabrication of self-organized TiO2nts and their
applications, the use of TiO2nts /Ti grid as anode material has never been investigated with a polymer
electrolyte to achieve the fabrication of all-solid-state microbatteries. To improve the performance of
the TiO2nts anodes for Li-ion microbatteries, self-organized TiO2nts grown on Ti grid is considered as
a great choice owing to its large aspect ratio of length to diameter, higher surface area and high Ti
conversion into TiO2nts [33,34]. Hence, the self-organized TiO2nts anode provides more easily access
for the Li ions, which improves the electrochemical performance of the microbatteries. Herein, we
report the fabrication of a liquid-free microbattery using self-organized TiO2nts/Ti grid filled by an
electropolymerized electrolyte. The effect of the anodic oxidation time on the formation of the TiO2nts
were investigated by scanning electron microscopy and the electrochemical performances of the
electropolymerized TiO2nts was also studied by cyclic voltammetry and galvanostatic
charge/discharge cycling. Compared to planar Ti surfaces (i.e. foil and thin film), we confirm that the
discharge capacity values obtained from TiO2nts supported on a Ti grid are strongly enhanced.

71

72
## 2. Experimental

### 2.1. Synthesis of TiO₂ nanotubes

The TiO₂nts anodes were fabricated by the electrochemical anodization of a titanium grid (Good Fellow 0.57 mm thickness, 0.23 mm wire diameter). Before anodization, the Ti grids were cut to 1.3 x 1.3 cm² in size and cleaned via sonication in acetone, isopropanol and methanol for 10 min each in order to remove any surface impurity. After drying the grids with compressed air, TiO₂nts were grown by the anodization of Ti grid in an organic electrolyte containing 96.7 wt. % glycerol, 1.3 wt. % NH₄F and 2 wt. % water [35]. All the anodization experiments were carried out at room temperature in a two-electrode system with a Ti grid as a working electrode and platinum (Pt) foil as a counter electrode. The working electrode was pressed against an O-ring of the electrochemical cell leaving approximately 0.63 cm² exposed to the electrolyte. The distance between the working and counter electrodes was set to 2 cm and the anodization was performed at room temperature without stirring of the electrolyte during anodization. A constant voltage of 60 V was applied to the two-electrode electrochemical cell using a generator (ISO-TECH IPS-603) for 1, 1.5, 2.5 and 3 h, respectively. After anodization, the samples were dipped in 0.5 vol. % HF solution for 30 seconds in order to remove the residue of the electrolyte, washed with distilled water and dried using compressed air. The as-formed TiO₂nts were annealed at 450 °C in air for 3 h with a heating rate of 5 °C min⁻¹ in order to obtain anatase phase.

### 2.2. Electrochemical polymerization

In order to achieve the electrodeposition of PMMA-PEG (poly methyl ether methacrylate-polyethylene glycol) polymer electrolyte, cyclic voltammetry was performed on the TiO₂nts in a three-electrode system using a VersaSTAT 3 potentiostat (Princeton Applied Research), Ag/AgCl as the reference and Pt electrode as the counter electrode in an aqueous solution composed of 0.5 M of bis(trifluoromethanesulfone)imide (LiTFSI) and 0.5 M MMA-PEG (methyl ether methacrylate-
polyethylene glycol) with an average molecular weight of 500 g mol⁻¹. Prior to electropolymerization, the aqueous solution containing the polymer electrolyte was purged with Argon gas for 10 min to remove dissolved oxygen. The cyclic voltammetry experiments were carried out for 100 cycles at the scan rate of 10 mV s⁻¹ in the potential window of -0.35 V to -1 V vs. Ag/AgCl (saturated) [20,36].

## 2.3. Characterizations

The crystallinity of the synthesized samples was examined by X-ray diffraction (XRD). The XRD pattern was recorded at room temperature using a Siemens D5000 diffractometer equipped with copper anticathode (Cu Kα radiation of 0.1506 nm wavelength was used with graphite monochromator). The diffractogramms were analyzed by comparing with the JCPDS-ICDD database (Joint Committee on Powder Diffraction Standards International Centre for Diffraction Data). The morphology of TiO₂nts was investigated by scanning electron microscopy (SEM) using a Carl Zeiss AG - ULTRA 55 SEM using an electron beam energy of 15 kV. The chronoamperometric test took place in a two-electrode electrochemical cell with Ti grid and Pt foil as a working and counter electrode, respectively, using PARSTAT 2273.

The Swagelok test cells were assembled in an Ar-filled glove box. In the half-cell system, TiO₂nts electrodes were assembled against metallic Li foil using the gel electrolyte of the LiTFSI and MMA-PEG. The Li foil was cut in a circular shape with the diameter of 9 mm and 2 circular sheets (10 mm in diameter) of the gel electrolyte in the Whatman paper were used as separator. The cells were galvanostatically charged and discharged in the potential window of 1 – 3 V vs. Li/Li⁺ at different current densities and cyclic voltammetry was performed at a scan rate of 0.1 mV s⁻¹ using a VMP3 potentiostat-galvanostat (Bio Logic).

117

118
## 3. Results and Discussion

In this work, the growth of TiO₂ nanotubes was carried out by a low-cost and simple electrochemical anodization of Ti grid at different anodization time in a glycerol electrolyte containing fluoride ions and small amounts of water. **Figure 1a** shows the actual size of Ti grid used in the experiments and the inset shows the SEM image of the Ti grid. It can be seen Ti grid consist of many thin and radial Ti filaments which increase the surface area of the substrate. **Figure 1b** shows the chronoamperometric curve of Ti grid anodized at 60 V for 3 h. As seen, after a minor increase at the beginning of the anodization, the current density dropped with time due to the presence of an electrical barrier formed by the compact oxide layer. The minor increase in current density at the early stage of anodization might be attributed to the exposure of surface area that was not covered with the electrolyte due to the nature of the Ti grid structure. Self-organized TiO₂nts starts to form as the result of the competition between electrochemical oxide formation and chemical dissolution of the oxide layer by fluoride ions according to **Equations 1 and 2**, respectively. Finally, steady current density was achieved when equilibrium was established between the growth and dissolution of the oxide layers [11].

$$ Ti + 2 H_2O \rightarrow TiO_2 + 4 H^+ + 4 e^- \quad (1) $$

$$ TiO_2 + 4 H^+ + 6 F^- \rightarrow TiF_6^{2-} + 2 H_2O \quad (2) $$

The crystallinity of the TiO₂nts was examined by XRD, as represented in **Figure 1c**. Immediately after growth the TiO₂nts the tubes are amorphous and the formation of the anatase phase is obtained after annealing treatment. The presence of new peaks at about 25.3° and 47.9° correspond to the reflections of anatase phase (JCPDS file no. 21-1272). The Ti peaks observed on the XRD analysis are Ti substrate due to the direct growth of TiO₂nts on the Ti grid. The residual Ti grid is directly used as the current collector.
<figure><img src="image_2.png" /></figure>

<figure><img src="image_3.png" /></figure>

<figure><img src="image_4.png" /></figure>

142

143

144

**Figure 1** a) Ti grid (inset: SEM image of Ti grid), b) chronoamperometric curve for the anodized Ti grid at applied potential of 60 V, and c) XRD patterns of TiO₂nts annealed in air at 450 °C for 3 h.

145

146

In this work, effects of anodization time on the formation of TiO2nts arrays have been investigated.

147

148

**Figure 2a-d** illustrates how the morphology and length of the anodized layer evolve with the anodizing time. The SEM images show the top surface and cross-section morphologies of TiO2nts anodized at 60

149

V for different durations of 1, 1.5, 2.5, and 3 h, respectively.
<figure><img src="image_5.png" /><figcaption>**Figure 2** SEM images of TiO₂ nanotube arrays formed by electrochemical anodization of the Ti grid at 60 V for 1 h (a), 1.5 h (b), 2.5 h, (c), and 3 h (d). Insets show the cross-sectional views.</figcaption></figure>

As seen, some changes can be observed with the increasing anodization time. For the shortest duration (1 h), the nanotubes are clearly visible and the length of the nanotubes is ca. 1.75 ± 0.1 µm (**Figure 2a**). However, the nanotube tops are not enough homogenous and smooth to ensure the conformal deposition of the polymer electrolyte. In **Figure 2b**, the SEM images showed the nanotubes anodized
for 1.5 h has an open-top structure without any bundle formation. The anodized Ti grid had comparatively longer and well-defined nanotubes, which are stable, well adherent to the grid substrate with a tube length of 1.9 ± 0.1 µm. Comparatively, 1.5 h and 1 h anodization does not show any bundle formation, yet, 1 h anodization showed shorter nanotubes than 1.5 h anodization. Indeed the collapse due to over dissolution of the top surface of nanotubes becomes very significant after 1.5 h. As a consequence, a substantial change in the morphology will affect the electrochemical performance of the electrodes. It is also observed that the length of the TiO2nts varies with the anodization time. The length of the TiO2nts increases as the anodization time **increases** from 1 h to 1.5 h, afterwards the length does not continue to increase with longer anodization time.

After longer anodization time (2.5 and 3 h), the nanotubes have closed-top structure and the bundled formation is found covering the entire top surface of the nanotubes. The thickness of the nanotubes layer after 2.5 h and 3 h anodization are 1.8 ± 0.2 µm and 1.5 ± 0.2 µm, respectively. Some studies showed that in long-duration anodization experiments, tubes can have inhomogeneous structures due to etching **of the top** [37]. The bundles on the tube tops might be formed due to the formation of needle-like morphologies as the walls may become too thin to support their own weight [11,38]. This bundle morphology is also described as nanograss or nanospike [39,40].

Nevertheless, **when the anodization time is decreased**, the **bundle formation** is disappeared. So, an appropriate oxidation time is the essential condition for the fabrication of highly ordered TiO₂ nanotube arrays onto Ti grid. These findings are in good agreement with the previous report. **Mor et al. reported** that the nanotubes can grow longer by extending the anodization time, however the top of the nanotubes are gradually destroyed after extended anodization. The partial collapse of the nanotubes occurred due to an over dissolution reaction of the tubes top during the prolonged anodization, leading to the formation of bundled nanotubes [41,42]. Also, Zeng et al. reported that TiO₂ nanotubes grown on Ti grid showing a well-defined nanotubular structure after 20 minutes anodization, however the tubes top
become fuzzy after prolonging the anodization time to 40 minutes [25]. Liu et al. [43] investigated the effect of the anodization time on the growth of TiO₂ nanotubes onto Ti grid at 60 V for 1-16 h and reported that the nanotube arrays grew uniformly after 3 h anodization. Additionally, as seen in Figure 2, several fissures and bundling on the surfaces of the nanotubes could also be attributed to van der Waals attraction and capillary forces during drying [11,26,34].

Indeed, compared to Ti foils substrate, the intertwined structure of the Ti grid had more promising results in terms of surface area. As a result, the electrolyte can penetrate easily to the entire surface of the nanotubes that are radially grown in a 3-D array on the Ti grid [43,44]. Therefore, to further study the electrochemical performance of the self-organized TiO₂nts/Ti grid, the TiO₂nts/Ti grid anodized for 1.5 h was selected to be studied as anode for all-solid-state Li-ion microbatteries using PMMA-PEG polymer electrolyte.

After growing the TiO₂nts on Ti grid substrate, the conformal electrodeposition of the electrolyte into nanotubes was achieved by the cyclic voltammetry (CV) technique. This approach is highly valuable to fully exploit the large surface area offered by the nanotubes through the formation of an augmented electrode/electrolyte interface [45-49]. **Figure 3** shows the cyclic voltammogram of the electropolymerization of the polymer electrolyte on the TiO₂nts. The window of the applied cathodic potential was selected between the H₂ bubbling and the beginning of the proton reduction (-1 V < E < E(H⁺/H₂) = -0.551 V vs. Ag/AgCl calculated from the Nernst equation) [46]. From cyclic voltammograms (CVs), as seen in **Figure 3a**, the absolute value of the cathodic current at -1 V vs. Ag/AgCl drops gradually with the increasing of cycles. The fading in the current can be explained by the successive deposition of the thin polymer layers that passivated the TiO₂nts electrode. Additionally, the redox peaks of Ti⁴⁺/Ti³⁺ are not observed and it is expected that there is no irreversible change in the oxidation states of Ti during the electropolymerization reaction. By using the same electrodeposition technique on the TiO₂nts/Ti foil, Plylahan et. al. [47] reported that after 5 cycles CV,
206 the growth of a polymer layer occurred inside and outside of each nanotube walls. Indeed, after 10
207 cycles CV, the inter-tube spaces are filled with the polymer and the nanotube walls become
208 significantly thicker compared to the sample obtained after 5 cycle of CV. After 100 cycles, the
209 polymer fills the inter-tube spaces and coats top surfaces of the TiO2nts/Ti grid (Figure 3b).

<figure><img src="image_6.png" /></figure>

210

211 **Figure 3 a)** Cyclic voltammograms of TiO2nts electrode in 0.5M LiTFSI + 0.5M MMA-PEG500. The curves were recorded in the potential window of -0.35 to -1 V vs. Ag/AgCl (3M) at the scan rate of 10 mV s⁻¹, **b)** SEM images of the bare TiO2nts for 1.5 h and electropolymerized TiO2nts (inset).

214

215 The CV experiments were performed to investigate the redox potential of TiO2nts electrodes. The CV
216 curves were recorded at the scan rate of 0.1 mV s⁻¹ between 1 and 3 V vs. Li/Li⁺. **In Figure 4a,** the two
217 curves exhibit well-defined cathodic and anodic peaks at 1.75 and 1.98 V vs. Li/Li⁺, respectively,
218 corresponding to lithium insertion/extraction potentials in anatase TiO2nts. The Li insertion/extraction
219 process is reversible as seen in the unchanged shape of the CV curves upon cycling. The consecutive
220 decrease in the absolute cathodic current indicates the slight discharge capacity fading upon cycling.

221 **Figure 4b** shows the galvanostatic charge/discharge profiles of the anatase TiO2nts. The profiles of
each sample show flat plateaus of charge at 1.77 V vs. Li/Li⁺ and discharge 1.88 V vs. Li/Li⁺ which are typical profiles for the anatase TiO₂nts.

<figure><img src="image_7.png" /><figcaption>**Figure 4.** a) Cyclic voltammogram of anatase phase TiO₂nts recorded at a scan rate of 0.1 mV s⁻¹ in the potential window of 1 V–3 V vs. Li/Li⁺, b) Galvanostatic charge/discharge profiles of the polymer-coated TiO₂nts electrode, c) Capacity vs. cycle number of the polymer-coated TiO₂nts electrode and d) Coulombic efficiency (%) the polymer-coated TiO₂nts electrode.</figcaption></figure>

The cycling performance of anatase TiO₂nts using the MMA-PEG500 gel electrolyte at C/10 and C/5 rates are displayed in **Figure 4**. The areal capacities were calculated considering a density of anatase (4.23 g cm⁻³), a nanotube layer thickness (1.8 ± 2 µm) and an estimated porosity of 50% [36,50]. The
233 cell cycled between 1 and 3 V vs Li/Li⁺ delivers an average capacity of ~376 µAh cm⁻² at C/10 and
234 ~350 µAh cm⁻² at C/5. The initial charge and discharge capacities of the electrodes are 375 µAh cm⁻²
235 and 580 µAh cm⁻², corresponding to a relatively low initial coulombic efficiency of 64.7%. A large
236 irreversible capacity observed at the first cycles is attributed to the side reaction of Li⁺ and the presence
237 of residual water at the surface of TiO₂nts and in the polymer electrolyte. Additionally, some Li ions
238 are trapped inside the TiO₂ lattice structure after the first Li⁺ insertion, thereby reducing the capacity
239 of the cell [35]. Nevertheless, for the subsequent cycles the capacities can be stabilized, the discharge
240 capacity values recorded in the 2nd and 3rd cycles are 382 and 380 µAh cm⁻² with improved coulombic
241 efficiency of 98.4 % and 98.7%, respectively. The cycling retention continuously enhanced after first
242 cycle and the coulombic efficiency approaches 100%.

243 The electrochemical performances of TiO2nts grown on Ti grid and Ti foil are summarized in **Table** 1. After 10 cycles, the storage capacity of the TiO2nts/Ti grid is fifteen times higher compared to our previous report with Ti foils [14]. Calculated using a microbattery voltage of 1.8 V, the obtained areal energy and power density of the TiO2nts/ Ti grid anode are 677 µWh cm⁻² and 67.7 µW cm⁻², respectively.

<table><caption>248 **Table 1.** Electrochemical performances of the microbatteries using PMMA-PEG polymer electrolyte</caption><thead><tr><th>Electrodes</th><th>Areal<br>Capacity at<br>C/10 rate after<br>10 cycles<br>(µAh cm<sup>-2</sup>)</th><th>Vcell<br>(V)</th><th>Energy<br>density<br>(µWh cm<sup>-2</sup>)</th><th>Power<br>density<br>(µW cm<sup>-2</sup>)</th></tr></thead><tbody><tr><td>TiO<sub>2</sub>nts/ Ti foil [20]</td><td>25</td><td>1.7</td><td>43</td><td>4.3</td></tr><tr><td>TiO<sub>2</sub>nts/ Ti grid</td><td>376</td><td>1.8</td><td>677</td><td>67.7</td></tr></tbody></table>

249

250

251
## 4. Conclusion

To sum up, Ti grid is used as a 3D substrate to form self-organized TiO₂ nanotubes. The anodization time shows a significant influence on the morphological properties of the nanotubes. Well-defined nanotubes without bundle formation with a tube length of 1.9 ± 0.1 µm can be obtained after 1.5 h anodizing a Ti grid. Due to its radial and intertwined structure, Ti grid supplies much larger area than a Ti foil for a same footprint area. Actually, Ti grid showed much higher areal capacity in comparison to Ti foil at the same kinetics (C/10 and C/5). The main reason is because self-supported nanotubes are successfully formed within a very large surface area increasing the amount of the active material and the battery performance. After 10 cycles, the storage capacity of the TiO₂nts/Ti grid is fifteen times higher compared to our previous report with Ti foils.

## Author Contribution

VA S performed experiments, analyzed the experimental results and wrote the manuscript. VA S, AG, APK, FV and TD discussed experimental results. FV and TD supervised the works. All the authors contributed to the reading of paper and gave advice on the revision of the manuscript.

## Conflict of Interest Statement

The authors declare that the research was conducted in the absence of any commercial or financial relationships that could be construed as a potential conflict of interest.

## Acknowledgment

We acknowledge Région Sud for the financial support.

## References

1. Baggetto L, Knoops HCM, Niessen RAH, Kessels WMM, Notten PHL. 3D negative electrode stacks for integrated all-solid-state lithium-ion microbatteries. *J Mater Chem* (2010) **20**:3703–3708.
278 2. Armand M, Tarascon J-M. Building better batteries. *Nature* (2008) **451**:652–657.

279 3. Sugiawati VA, Vacandio F, Eyraud M, Knauth P, Djenizian T. Porous NASICON-Type Li3Fe2(PO4)3 Thin Film Deposited by RF Sputtering as Cathode Material for Li-Ion Microbatteries. *Nanoscale Res Lett* (2016) **11**.

282 4. Sugiawati VA, Vacandio F, Knauth P, Djenizian T. Sputter-Deposited Amorphous LiCuPO4 Thin Film as Cathode Material for Li-ion Microbatteries. *ChemistrySelect* **3**:405–409. doi:10.1002/slct.201702429

285 5. Ferrari S, Loveridge M, Beattie SD, Jahn M, Dashwood RJ, Bhagat R. Latest advances in the manufacturing of 3D rechargeable lithium microbatteries. *J. Power Sources* (2015) **286**:25–46.

287 6. Nasreldin M, Delattre R, Ramuz M, Lahuec C, Djenizian T, de Bougrenet de la Tocnaye J-L. Flexible Micro-Battery for Powering Smart Contact Lens. *Sensors* (2019) **19**:2062.

289 7. Zheng S, Wu Z-S, Zhou F, Wang X, Ma J, Liu C, He Y-B, Bao X. All-solid-state planar integrated lithium ion micro-batteries with extraordinary flexibility and high-temperature performance. *Nano Energy* (2018) **51**:613–620.

292 8. Oudenhoven JFM, Baggetto L, Notten PHL. All-Solid-State Lithium-Ion Microbatteries: A Review of Various Three-Dimensional Concepts. *Adv. Energy Mater.* (2011) **1**:10–33.

294 9. Jaroenworaluck A, Regonini D, Bowen CR, Stevens R, Allsopp D. Macro, micro and nanostructure of TiO2 anodised films prepared in a fluorine-containing electrolyte. *J. Mater. Sci.* (2007) **42**:6729–6734.

297 10. Fraoucene H, Sugiawati VA, Hatem D, Belkaid MS, Vacandio F, Eyraud M, Pasquinelli M, Djenizian T. Optical and Electrochemical Properties of Self-Organized TiO2 Nanotube Arrays From Anodized Ti–6Al–4V Alloy. *Front Chem.* (2019) **7**.

300 11. Roy P, Berger S, Schmuki P. TiO2 nanotubes: Synthesis and applications. *Angew. Chem. Int. Ed.* (2011) **50**:2904–2939.

302 12. Krysa J, Lee K, Pausova S, Kment S, Hubicka Z, Ctvrtlik R, Schmuki P. Self-organized transparent 1D TiO2 nanotubular photoelectrodes grown by anodization of sputtered and evaporated Ti layers: A comparative photoelectrochemical study. *Chem.Eng. J.* (2017) **308**:745–753.

306 13. Galstyan V, Vomiero A, Comini E, Faglia G, Sberveglieri G. TiO2 nanotubular and nanoporous arrays by electrochemical anodization on different substrates. *RSC Adv.* (2011) **1**:1038–1044.

308 14. Assefpour-Dezfuly M, Vlachos C, Andrews EH. Oxide morphology and adhesive bonding on titanium surfaces. *J. Mater. Sci.* (1984) **19**:3626–3639.

310 15. Zwilling V, Darque-Ceretti E, Boutry-Forveille A, David D, Perrin MY, Aucouturier M. Structure and physicochemistry of anodic oxide films on titanium and TA6V alloy. *Surf. Interface Anal.* (1999) **27**:629–637.
313
314
315

16. Zhou X, Liu N, Schmuki P. Photocatalysis with TiO2 Nanotubes: “Colorful” Reactivity and Designing Site-Specific Photocatalytic Centers into TiO2 Nanotubes. *ACS Catal.* (2017) **7**:3210–3235.

316
317
318

17. Galstyan V, Comini E, Baratto C, Ferroni M, Poli N, Faglia G, Bontempi E, Brisotto M, Sberveglieri G. Two-phase Titania Nanotubes for Gas Sensing. *Procedia Eng.* (2014) **87**:176–179.

319
320

18. Shankar K, Mor GK, Prakasam HE, Varghese OK, Grimes CA. Self-Assembled Hybrid Polymer–TiO2 Nanotube Array Heterojunction Solar Cells. *Langmuir* (2007) **23**:12445–12449.

321
322

19. Ellis BL, Knauth P, Djenizian T. Three-Dimensional Self-Supported Metal Oxides for Advanced Energy Storage. *Adv. Mater.* (2014) **26**:3368–3397.

323
324
325

20. Plylahan N, Letiche M, Samy Barr MK, Ellis B, Maria S, Phan TNT, Bloch E, Knauth P, Djenizian T. High energy and power density TiO2 nanotube electrodes for single and complete lithium-ion batteries. *J. Power Sources* (2015) **273**:1182–1188.

326
327

21. Macák JM, Tsuchiya H, Schmuki P. High-aspect-ratio TiO2 nanotubes by anodization of titanium. *Angew. Chem. Int.Ed.* (2005) **44**:2100–2102. doi:10.1002/anie.200462459

328
329
330

22. Sopha H, Salian GD, Zazpe R, Prikryl J, Hromadko L, Djenizian T, Macak JM. ALD Al2O3-Coated TiO2 Nanotube Layers as Anodes for Lithium-Ion Batteries. *ACS Omega* (2017) **2**:2749–2756.

331
332
333

23. Salian GD, Krbal M, Sopha H, Lebouin C, Coulet M-V, Michalicka J, Hromadko L, Tesfaye AT, Macak JM, Djenizian T. Self-supported sulphurized TiO2 nanotube layers as positive electrodes for lithium microbatteries. *Appl. Mater. Today* (2019) **16**:257–264.

334
335
336

24. Salian GD, Koo BM, Lefevre C, Cottineau T, Lebouin C, Tesfaye AT, Knauth P, Keller V, Djenizian T. Niobium Alloying of Self-Organized TiO2 Nanotubes as an Anode for Lithium-Ion Microbatteries. *Adv. Mater. Technol.* (2018) **3**:1700274.

337
338

25. Zeng Q-Y, Xi M, Xu W, Li X-J. Preparation of titanium dioxide nanotube arrays on titanium mesh by anodization in (NH4)2SO4/NH4F electrolyte. *Mater. Corros.* (2013) **64**:1001–1006.

339
340

26. Gulati K, Santos A, Findlay D, Losic D. Optimizing Anodization Conditions for the Growth of Titania Nanotubes on Curved Surfaces. *J. Phys. Chem. C* (2015) **119**:16033–16045.

341
342

27. He W, Qiu J, Zhuge F, Li X, Lee J-H, Kim Y-D, Kim H-K, Hwang Y-H. Advantages of using Ti-mesh type electrodes for flexible dye-sensitized solar cells. *Nanotechnology* (2012) **23**:225602.

343
344
345

28. Chun KY, Park BW, Sung YM, Kwak DJ, Hyun YT, Park MW. Fabrication of dye-sensitized solar cells using TiO2-nanotube arrays on Ti-grid substrates. *Thin Solid Films* (2009) **517**:4196–4198.

346
347
348

29. Gerosa M, Sacco A, Scalia A, Bella F, Chiodoni A, Quaglio M, Tresso E, Bianco S. Toward Totally Flexible Dye-Sensitized Solar Cells Based on Titanium Grids and Polymeric Electrolyte. *IEEE J. Photovolt.* (2016) **6**:498–505.
349
350

30. Liu Z, Subramania V (Ravi), Misra M. Vertically Oriented TiO2 Nanotube Arrays Grown on Ti Meshes for Flexible Dye-Sensitized Solar Cells. *J. Phys. Chem. C* (2009) **113**:14028–14033.

351
352
353
354

31. Motola M, Dworniczek E, Satrapinskyy L, Chodaczek G, Grzesiak J, Gregor M, Plecenik T, Nowicka J, Plesch G. UV light-induced photocatalytic, antimicrobial, and antibiofilm performance of anodic TiO2 nanotube layers prepared on titanium mesh and Ti sputtered on silicon. *Chem. Pap* (2019) **73**:1163–1172.

355
356
357

32. Martin M, Leonid S, Tomáš R, Jan Š, Jaroslav K, Mariana K, Michaela J, František P, Gustav P. Anatase TiO2 nanotube arrays and titania films on titanium mesh for photocatalytic NOX removal and water cleaning. *Catal. Today* (2017) **287**:59–64.

358
359

33. Rustomji CS, Frandsen CJ, Jin S, Tauber MJ. Dye-Sensitized Solar Cell Constructed with Titanium Mesh and 3-D Array of TiO2 Nanotubes. *J. Phys. Chem. B* (2010) **114**:14537–14543.

360
361
362

34. Liao J, Lin S, Zhang L, Pan N, Cao X, Li J. Photocatalytic Degradation of Methyl Orange Using a TiO2/Ti Mesh Electrode with 3D Nanotube Arrays. *ACS Appl. Mater. Interfaces* (2012) **4**:171–177.

363
364

35. Ozkan S, Nguyen NT, Mazare A, Cerri I, Schmuki P. Controlled spacing of self-organized anodic TiO2 nanotubes. *Electrochem. Commun.* (2016) **69**:76–79.

365
366

36. Plylahan N, Letiche M, Barr MKS, Djenizian T. All-solid-state lithium-ion batteries based on self-supported titania nanotubes. *Electrochem. Commun.* (2014) **43**:121–124.

367
368

37. Macak JM, Tsuchiya H, Taveira L, Aldabergerova S, Schmuki P. Smooth anodic TiO2 nanotubes. *Angew. Chem. Int. Ed.* (2005) **44**:7463–7465.

369
370

38. Macak JM, Schmuki P. Anodic growth of self-organized anodic TiO2 nanotubes in viscous electrolytes. *Electrochim. Acta* (2006) **52**:1258–1264.

371
372
373

39. Song Y-Y, Lynch R, Kim D, Roy P, Schmuki P. TiO2 Nanotubes: Efficient Suppression of Top Etching during Anodic Growth Key to Improved High Aspect Ratio Geometries. *Electrochem Solid-State Lett.* (2009) **12**:C17–C20.

374
375

40. Kirchgeorg R, Kallert M, Liu N, Hahn R, Killian MS, Schmuki P. Key factors for an improved lithium ion storage capacity of anodic TiO2 nanotubes. *Electrochim. Acta* (2016) **198**:56–65.

376
377
378

41. Mor GK, Varghese OK, Paulose M, Shankar K, Grimes CA. A review on highly ordered, vertically oriented TiO2 nanotube arrays: Fabrication, material properties, and solar energy applications. *Sol. Energ. Mat. Sol. C.* (2006) **90**:2011–2075.

379
380
381

42. Altomare M, Pozzi M, Allieta M, Bettini LG, Selli E. H2 and O2 photocatalytic production on TiO2 nanotube arrays: Effect of the anodization time on structural features and photoactivity. *Appl. Catal. B: Environmental* (2013) **136–137**:81–88.

382
383

43. Liu Z, Zhang Q, Zhao T, Zhai J, Jiang L. 3-D vertical arrays of TiO2 nanotubes on Ti meshes: Efficient photoanodes for water photoelectrolysis. *J. Mater. Chem* (2011) **21**:10354–10358.
384
385
386

44. Zhang Z-J, Zeng Q-Y, Chou S-L, Li X-J, Li H-J, Ozawa K, Liu H-K, Wang J-Z. Tuning three-dimensional TiO2 nanotube electrode to achieve high utilization of Ti substrate for lithium storage. *Electrochim. Acta* (2014) **133**:570–577.

387
388
389

45. Ferrari IV, Braglia M, Djenizian T, Knauth P, Di Vona ML. Electrochemically engineered single Li-ion conducting solid polymer electrolyte on titania nanotubes for microbatteries. *J Power Sources* (2017) **353**:95–103.

390
391
392
393

46. Salian GD, Lebouin C, Demoulin A, Lepihin MS, Maria S, Galeyeva AK, Kurbatov AP, Djenizian T. Electrodeposition of polymer electrolyte in nanostructured electrodes for enhanced electrochemical performance of thin-film Li-ion microbatteries. *J Power Sources* (2017) **340**:242–246.

394
395
396

47. Plylahan N, Maria S, Phan TN, Letiche M, Martinez H, Courrèges C, Knauth P, Djenizian T. Enhanced electrochemical performance of Lithium-ion batteries by conformal coating of polymer electrolyte. *Nanoscale Res. Lett.* (2014) **9**:544.

397
398
399

48. Sugiawati VA, Vacandio F, Ein-Eli Y, Djenizian T. Electrodeposition of polymer electrolyte into carbon nanotube tissues for high performance flexible Li-ion microbatteries. *APL Mater.* (2019) **7**:031506.

400
401
402

49. Braglia M, Ferrari IV, Djenizian T, Kaciulis S, Soltani P, Di Vona ML, Knauth P. Bottom-Up Electrochemical Deposition of Poly(styrene sulfonate) on Nanoarchitected Electrodes. *ACS Appl. Mater. Interfaces* (2017) **9**:22902–22910.

403
404
405

50. Plylahan N, Letiche M, Samy Barr MK, Ellis B, Maria S, Phan TNT, Bloch E, Knauth P, Djenizian T. High energy and power density TiO2 nanotube electrodes for single and complete lithium-ion batteries. *J Power Sources* (2015) **273**:1182–1188.

406
407
408

51. Ortiz GF, Hanzu I, Djenizian T, Lavela P, Tirado JL, Knauth P. Alternative Li-Ion Battery Electrode Based on Self-Organized Titania Nanotubes. *Chem Mater* (2009) **21**:63–67.

409
<figure><img src="image_8.png" /><figcaption>Figure 1.TIF</figcaption></figure>

<figure><img src="image_9.png" /></figure>

<figure><img src="image_10.png" /></figure>
<figure><img src="image_11.png" /><figcaption>Figure 2.TIF</figcaption></figure>
<figure><img src="image_12.png" /><figcaption>Figure 3.TIF</figcaption></figure>

In review
<figure><img src="image_13.png" /><figcaption>Figure 4.TIF</figcaption></figure>

<figure><img src="image_14.png" /></figure>

<figure><img src="image_15.png" /></figure>

<figure><img src="image_16.png" /></figure>
<figure><img src="image_17.png" /><figcaption>Figure 6.TIF</figcaption></figure>

<figure><img src="image_18.png" /></figure>

<figure><img src="image_19.png" /></figure>
<figure><img src="image_20.png" /><figcaption>Figure 7.TIF</figcaption></figure>
<figure><img src="image_21.png" /><figcaption>Figure 8.TIF</figcaption></figure>

In review
<figure><img src="image_22.png" /><figcaption>Figure 9.TIF</figcaption></figure>

<figure><img src="image_23.png" /></figure>

<figure><img src="image_24.png" /></figure>

<figure><img src="image_25.png" /></figure>